Co(II) Coordination Polymers: Positional Isomeric Effect, Structural and Magnetic Diversification
Huang, Fu-Ping; Tian, Jin-Lei; Gu, Wen; Liu, Xin; Yan, Shi-Ping; Liao, Dai-Zheng; Cheng, Peng; Crystal Growth & Design 10 (2010) 1145–; doi:10.1021/cg901014r

data_4502347
_publ_section_title
;
 Co(II) Coordination Polymers: Positional Isomeric Effect, Structural and
 Magnetic Diversification
;
_journal_issue                   3
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              1145
_journal_paper_doi               10.1021/cg901014r
_journal_volume                  10
_journal_year                    2010
_chemical_formula_sum            'C28 H23 Co2 N7 O16'
_chemical_formula_weight         831.39
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                112.95(3)
_cell_angle_beta                 90.96(3)
_cell_angle_gamma                102.69(3)
_cell_formula_units_Z            2
_cell_length_a                   11.269(2)
_cell_length_b                   11.987(2)
_cell_length_c                   12.723(3)
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.50
_cell_volume                     1533.9(7)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0652
_diffrn_reflns_av_sigmaI/netI    0.0801
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            13233
_diffrn_reflns_theta_full        25.50
_diffrn_reflns_theta_max         25.50
_diffrn_reflns_theta_min         3.06
_exptl_absorpt_coefficient_mu    1.175
_exptl_absorpt_correction_T_max  0.868
_exptl_absorpt_correction_T_min  0.754
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    1.800
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             931
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.12
_refine_diff_density_max         0.441
_refine_diff_density_min         -0.384
_refine_diff_density_rms         0.085
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.130
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     502
_refine_ls_number_reflns         5669
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.130
_refine_ls_R_factor_all          0.0983
_refine_ls_R_factor_gt           0.0656
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0419P)^2^+0.7290P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1175
_refine_ls_wR_factor_ref         0.1289
_reflns_number_gt                4252
_reflns_number_total             5669
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg901014r_si_007.cif
_cod_data_source_block           aa
_cod_original_cell_volume        1533.8(5)
_cod_original_sg_symbol_H-M      p-1
_cod_database_code               4502347